dL dZ2 dZ1dt dt dtdVF2 dZ 2 dZR10 R20dt dt dtdg0dt1 2if growing at 1-end (dZ 1 /dt>0)if not growing at 1-end (dZ 1 /dt
83. APPLICATION TO THE CASE OF GROWING FROM A NEARLY-SQUAREBARConsider an initially near-square bar (of uniform cross-section) of raw solid material, defined by its meanradius R i0 (e.g. R i0 =5 mm) and C i4 /R i0 =0.14 (the first coefficient of the Fourier cosine-expansion of asquare). If the figure-of-merit for "squareness" is defined by the ratio of the area of the inscribed square tothe area of the whole cross-section, a circle has a ratio of 2/=0.63, whereas with the fist harmonic it goesup to 0.95. To better grasp how much square the first harmonic gives, Fig. 3a shows the whole crosssection,but in Fig. 3b only two meridian cuts are shown: R =0 (i.e. maximum radii) and R =/4 (i.e.minimum radii). In the figures to follow, only these two radial profiles are used to visualise the 3D-shapein 2D plots.Fig. 3. Initial near-square solid bar in units of its mean radius R 1 : a) whole cross-section, b) only twomeridian cuts are shown: R(0)/R 1 (i.e. maximum radii, solid line) and R(/4)/R 1 (i.e. minimumradii, dash line). In the figures to follow, only these two radial profiles are used to visualise the3D-shape in 2D plots.Consider that a certain length L of this bar has been molten and assume that this is really the initial statefrom which crystal growth is to be simulated. The initial liquid interface is found from Eq. (22) andplotted in Fig. 4a for the cases of L/(2R 1 )=1 and two values of axial gravity, corresponding to B=0 andB=1; in this case, this large Bond value is still acceptable for the linear analysis of short liquid bridge (in arecent review  of the hydrostatics of liquid bridges with several loads, it can be seen that the maximumBond value for the present geometry is larger than 2). The 8% volume reduction upon melting for silicongrowth has been accounted for and can be clearly appreciated in the figure. To see the effect of non-equalinitial supports, Fig. 4b has been computed to show the initial molten shape between a near-square and aperfect circular support of different sizes (R 10 /R 20 =0.8/1.2, L/(R 10 +R 20 )=1. Observe that, in any case, thenon-axisymmetric effects only count near the non-circular ends, the liquid bridge tending to beaxisymmetric in mid lengths.ab11RR / 0RR / 00011RR / 0RR / 0010ZR / 01010ZR / 01
9Fig. 4 Initial molten shape of slenderness =L/(2R 0 )=1 of the bar in Fig. 3 (the two extreme meridiansshown, for =0 solid, and for =/4 dashed) for the case of zero gravity (upper) and for an axialgravity corresponding to B=1 (lower), in units of the mean radius R 0 . In b, the effect of non-equalends (a square one with R 10 /R 0 =0.8 and a circular one with R 20 /R 0 =1.2 is shown.Now the simulated crystal growth process may be started by considering some pulling-heating lawequivalent to, say, a growing rate of dZ 1 /dt=10 5 m/s and constant molten length dZ 2 /dt=dZ 1 /dt (forconstant length evolution), and an adequate time step for the discrete simulation (say t=10 s), irrelevantfor the physics being simulated. Some results are presented in Fig. 5, simulating the crystal growth from anearly-square silicon rod with a molten zone of aspect ratio =0.5 (Fig. 5a), =1 (Fig. 5b), and =2 (Fig.5c), without external loads (B=0). It can be seen how the 11º growth-angle for silicon (Fig. 2) tends toneck the solid grown. Although the molten length, material properties and applied loads are kept constantin the three series, the more slender one (=2) shows unstable growth (neck breaking will follow). In anycase, both the grown solid and the molten zone tend to be axisymmetric, with the non-axisymmetrylimited to the ends.Fig. 5. Simulated crystal growth from an initially near-square silicon bar of mean radius R 0 and aspectratio =0.5, 1 and 2, without external loads (B=0), where it can be seen how the 11º growth-angle(Fig. 2) tends to neck the solid grown.The maximum slenderness of the molten zone for stable crystal growth depends on the applied loads, andin Fig. 6 the stable limits in the case of a constant axial load (residual acceleration) is presented as afunction of the slenderness, for the initially near-square bar. The upper limit of stability in Fig. 6corresponds to the molten bridge necking near the melting front (with fat crystal growing), and the lowerlimit to the molten bridge necking near the solidification front (with narrowing crystal growth).
10Fig. 6. Limiting axial loads (measured by the Bond number, B) for stable crystal growth from an initialliquid bridge obtained by zone-melting in a near-square silicon bar of mean radius R 0 , in the caseof maintaining a constant molten length L. Growth shapes at a, b and c depicted in Fig. 7.To better appreciate the effect of an axial residual gravity on the growth and its stability, Fig. 7 has beenprepared by simulation of a floating zone process of constant molten length, =2, in an initially nearsquaresilicon bar, for the three loads corresponding to the three regions in Fig. 6: an axial load B=0.040in the middle of the stable region, and two unstable loads, B=0.010 and B=0.075, one at each side of thestability limits (check with Fig. 6).Fig. 7. Simulated crystal growth from an initially near-square silicon bar of mean radius R 0 , assuming afurnace control law such as to keep the molten length L constant all the time with =2,corresponding to the three cases marked in Fig. 6: axial loads B=+0.010 (a), B=+0.040 (b) andB=+0.075 (c), the middle one being the only stable growth.As said before, although most of the results here presented refer to an initial prismatic silicon bar with anear-square cross-section, the procedure here developed allows for any geometry of the end supports:unequal seed and feed sides, even eccentric, with the only bounds of the linear analysis based on thecylindrical geometry, that is for radial departures much smaller than the mean radius.CONCLUSIONSThe objective of this paper was to simulate the growing of crystals of non-circular cross-section by thefloating zone technique and analyse the sequence of shapes and their stability. This has been done byusing the hydrostatic liquid-bridge model (without any internal motions), shown in the literature to berepresentative of the mechanical behaviour in the real process.The simulation has been achieved by a mathematical model valid for shapes not too far from that of acylindrical molten zone. As an example, it has been applied to an initially near-square silicon bar, with aninitial departure from the mean cylinder of 14% to best approach a square cross-section, expecting anuncertainty in the results of the order of a few percent.As a general result, it has been found that there is a strong tendency for the liquid interface to get circular,and subsequently for the grown solid to get a circular cross-section, even if the initial rod is not of circularcross-section.
11Detailed results have been found for the maximum molten length allowing a stable growth (withoutnecking and bridge rupture) as a function of the residual axial gravity (measured by the Bond number).The algorithm developed could be directly applied to simulate the growth with different geometries anddifferent growth laws, within the linearised mathematical model.As a follow-on, a more closed-form analysis might be pursued, for instance to develop an analyticalexpression for the limits of stable growth as a function of the geometry and the loads, or a more appliednumerical simulation of the non-linear aspects (geometries far from the cylinder, large shapedeformations, and so on).ACKNOWLEDGEMENTSThis work has been supported by the Spanish Ministerio de Ciencia y Tecnología (MCYT).REFERENCES Lan, C.W., Kou, S.: "Shortened floating zone crystal growth under normal gravity". J. CrystalGrowth 119, 281,291 (1992). Cröll, A., Kaiser, T., Schweizer, M., Danilewsky, A.N., Lauer, S., Tegetmeier, A., and Benz, K.W.:"Floating-zone and floating-solution-zone growth of GaSb under microgravity". J. Crystal Growth191, 365, 376 (1998). Martínez, I., Cröll, A.: "Liquid bridges and floating zones". ESA SP-333, 135, 142 (1992). Martínez, I., Eyer, A.: "Liquid bridge analysis of silicon crystal growth experiments undermicrogravity". J. Crystal Growth 75, 535, 544 (1986). Boucher, E.A., Evans, M.J.B.: "A liquid-bridge model for the flat-zone processing of materials". J.Chem. Soc. Faraday Trans. I. 81, 2787, 2796 (1985). Martínez, I., Perales, J.M.: "Mechanical behaviour of liquid bridges in microgravity in Physics ofFluids in Microgravity". in "Physics of Fluids in Microgravity", R. Monti (Ed.), Taylor & Francis,pp. 21-45, (2001). Meseguer, J., Perales, J.M., Martínez, I., Bezdenejnykh, N.A., Sanz, A.: "Hydrostatic Instabilities inFloating Zone Crystal Growth Process". Current Topics in Crystal Growth Research 5, 27, 42(1999). Rossolenko, S.N., Zhdanov, A.V.: "Equilibrium shapes of liquid menisci subjected to gravity forceand surface tension". J. Crystal Growth 104, 8, 13 (1990). Pet'kov, I.S., Red'kin, B.S.: "Calculation of the stationary cross-section form of nonaxisymmetricalcrystals growing from the melt". J. Crystal Growth 131, 598, 606 (1993). Tatarchenko, V.A., Uspenski, V.S., Tatarchenko, E.V., Nobot, I.Ph., Duffar, T., Roux, B.:"Theoretical model of crystal growth shaping process". J. Crystal Growth 180, 615, 626 (1997). Hamidi, M., Rodot, H.: "Experimental determination of the growth angle: application to silicon".Revue de Physique Appliquée 18, 75, 80 (1983). Martínez, I., Sanz, A., Perales, J.M., Meseguer, J.: "Freezing of a Long Liquid Column on theTexus-18 Sounding Rocket Flight". ESA Journal 12, 483, 489 (1988). Bezdenejnykh, N.A., Meseguer, J..: "On the use of liquid bridges as accelerometers". MicrogravitySci. Technol. 9, 62, 69 (1996). Perales, J.M., Meseguer, J., Martinez, I.: "Minimum Volume of Axisymmetric Liquid Bridgesbetween Unequal Disks in an Axial Microgravity Field". J. Crystal Growth 110, 855, 861 (1991). Martinez, I, Meseguer, J., Perales, J.M.: "Analytical Modelling of Floating Zone Crystal Growth".Adv. Space Res. Vol. 29, No. 4, pp. 569-574 (2002).